A P~ENOMENOLOGICAL THEORY FOR PLASTIC OF POLYGRYSTALLINE METALS*
DEFORMATION
E. W. HART? A consistent phenomenologioal theory is developed for t,he plastic deformation properties of a restricted class of polycrystalline metals. The t,heory introduces the concept of a “hardness state” that can be related to the dislocation “structure” generated in the course of plastic deformation. The conditions t,hat must be satisfied if a plastia equation of state is t,o hold are investigated, and it’ is concluded that it is likely that such an equation of state exists. The implications for current microscopic theories are explored. Some of the current, conclusions that are drawn from experimental data are criticized. In particular, it is shown that the neglect of the influences of anelasticity and of grain boundary sliding has led to incorrect interpretations of grain matrix flow properties. Furthermore. the existence of a steady state deformation regime is challenged. THEORIE
PHESOMESOLOGTQUE
DE LA DEFORMATIOS POLYCRISTALLISS
PLaSTIQUE
DES
MET.4US
L’auteur presente une theorie phenomenologique coherente pour lea proprietds de la deformation La theorie introduit le concert. d’un plastique d’une categoric restreinte de meteus polycristallins. ‘*et& de durete” qui peut Btre relic it la “structure” des dislocations engendree au tours de la deformation plastique. L’auteur Qtudie les conditions a satisfaire pour qu‘une equat.ion d’Pt,at soit. valable clans ee eas, et il conclue qu’il est vraisemblable qu‘une telle equation esiste. I1 recherche les consequences sur les theories courantes macroscopiques. L’auteur critique certaines concfusions courantes qui sont tirees des result&s esperimentaus. En incorrectes des proprietes plast,iques particulier il montre qu’on arrive a des interpretations de la matrice des grains si on neglige l’influence de 1’anelast~ieit.Bet du glissement des joints de grains. En outre, l’existence d’un regime de deformation stationnaire est discut&. EINE
PHASOMESOLOGISCHE THEORIE POLYKRISTALLINER
DER PLASTISCHES METALLE
VERFGRBIUSG
Eine konsistent,e phlinomenologische Theorie der plastischen Verformung einer besohrankten Gruppe polykrjstalliner Metalle wird entwiokelt.. Die Theorie fiihrt einen “Hartezustand” ein, der mit, der im Verlauf der Verformung eneugten “Ve~etzungsstruktur.’ in Zu~mmenhang gebracht werden kann. Bedingungen, die erfiillt sein miissen. wenn eine plast.ische Zustandsgleichung gelten ~011. werden untersucht und es wird geschlossen, dal3 wahrscheinlich eine solche Zustandsgleichung esixticrt. Die Folgerungen fur vorhandene mikroskopische Theorien nerden behendelt. Einige der bisherigen Schlugfolgerungen aus experimentellen D&en werden kritisiert. Insbesondere wird gezeigt, dal3 die Vernachliissigung des Einflusses der Anelestizitat und der Korngrenzengleitung zur falsohen Interpretation der FlieDeigenschaften der Kornmatris gefiihrt hat. Aufierdem wirtl die Exintenz tines stat&hen Verformunpabereichs in Frage grstellt.
1. INTRODUCTION
The customary tion behavior
description
met*als will necessarily
of the plastic deforma
of metals consists largely of collections
of tensile stressstrain rates and creep curves
curves for several extension for a variet,y of loading con
This mode of descript,ion generally serves ditions. to emphasize that the flow rate at any given time
and attempts
appear t,o be rat,her capricious.
at theoretical
elucidation
hensive phenomenology for the facts of deformation behavior as distinct, from the present empiricism. The purpose of the present paper is to examine
under some applied load depends on the prior defor
current
mation history.
tive sohttion for a restricted,
The question naturally
it is possible to summarize instant
arises whether
the prior history
in terms of some readily measurable
at, any property
class of materials evident,
detailed
held views.
history.
If such a
procedure is t’o be really effect,ual. the entire descript.ion should be possible in terms of well defined deformation
variables.
* Received October 7, 1969.
t General Electric Research Schenectady, New York, U.S.A. METALLURGICA,
VOL.
and
Development
1X, JUXE
1970
Center,
It will become
is developed
below. that some
we shall make about t’he nature of areindisagreement
It will be concluded.
with commonl!
for example.
that
there is no clear evidence for a steady stat,e cleformat,ion regime. Clearly, such a conclusion is of considerable importance
It, should be noted that. if such a description is not possible, the phenomenon of plastic deformation of
ACTA
of the conclusions
but nevert,heless broad.
and phenomena.
as the theory
plastic deformation
of the prior
t.lw
state of this problem and to propose a tenta
of the mataerial so t,hat fut,ure deformation response can then be predicted independently of any more knowledge
of microscopic
mechanisms then will lack clearly defined goals. In other words what is desired is a reasonably compre
we emphasize tude
from a t,heoretical point of view. am1 it here simply to underline the magni
of the contrast
considered
that
only empirically
ganized into a consistent 599
is possible
between
and the same data
phenomenology.
data or
ACTA
600
METALLURGICA,
The plan of the paper is as follows: after briefly considering properties
2,
of the plastic
to the nature of the test data, the current
view will be described define the restrictions will introduce
and criticized.
deformation
Section
on the proposed
a definition
will be concerned
the possible
straining
4
relationships
data
needed
for a crucial
the conclusions
test of the
that have been
drawn from current load change experiments. ‘i will be devoted
to discussion
the phenomenology on microscopic
Section
of the relationship
to theories of deformation
of
based
The application
of a tensile stress u to a metal speci
of three
identifiable
components:
elastic strain E,. anelastic strain E, and plastic strain E,,. Ef = E, + E, + Ep. The time
dependence
that of
to describe
Ed
is determined
and is different
only
by
by relaxation
in character
from
by such load release.
distinguish
the
three
These cherac
strain
components
laws
that
are satisfied
components
are
fairly well understood.
of recoverable The
the
relatively
state aariables
n&Ural unstrained
by
simple
are
by the
E, and E, are good
of the material.
There is a
state relative to which the amount is rather
different
then,
significant
change
tion
either the same stress subsequent deformation
under
However,
by definition
with the
of steady
will accompany
strain rate must
result
state,
further
or strain rate. at a different
in an eventual
much strain was introduced
new steady
although
specimen
cannot
accumulated equation
the state
of strain
be described
strain,
of state”
simple.
of a
solely in terms of the
there
may
in somewhat
independent
to show
hardening exist
a
“plastic
more general terms
of state may
The existence of such an equation
furthermore,
on how
steady state.
at theinterim
It is the purpose of the present treatment that,
no
deforma
That latter steady state can have been reached
of whether
exists a steady state deformation
be rather of state is,
or not
there
rhgime.
3. THE
the
OF
STATE
deformation
histories at a single temperature
metals.
specimens
of
relatively
We exclude from consideration
and inhomogeneous
flow processes.
purport to describe the behavior a range sliding
of strain plays
importance
a
rates
role.
is the requirement only between
f.c.c.
discontinuous
Furthermore
we
of such specimens in
for which
negligible
and to
pure
grain Of
boundary
considerable
that we will consider
the stress and the plastic
strain.
The modifications
field
strain below.
components will be considered separately Since experimental observations measure all
reference state is
strain
need not even
with a single valued displacement
Even when an arbitrary
plastic
EQUATION
The theory to be presented here will be restricted to
relationships for
The plastic strain components
be compatible
and
strain can be measured.
situation
in general.
recoverable
They are characterized
fact that the st,rain components deformation
strain.
fact,
the state of strain hardening
is reached.
polycrystalline
uniquely. strain
Zenerin
The elastic and anelastic strain is recover
E,.
not recoverable
The
the
and.
This view is in contradiction
able after release of the stress Q, the plastic strain is teristics
works,
in terms of the amount of strain it has
and that such an equation
of E, is determined
that of E, and
and dissipation
temperature,
almost
changes
that, if all
then by different amounts of strain, depending
PROBLEM
men results in a total tensile strain Q that is in general time dependent. The accumulated total strain at any is the sum
be argued
equally commonly held point of view that there is a steady state regime, for certainl, if a “steady state”
state.
considerations. 2. THE
inertia;
customary undergone.
and examine
if temperature
common practice in describing deformation properties proceeds as though it did work. In other words, it is
are to be
Tn Section 6 we consider the nature of the
at one
treatment
Section 5 will show how predictions
experimental
time
is done
of a specimen
examples.
of Zener and Hollomon
It can probably
state be
the strain hardening
made with a theory of this type by meens of specific
theory
are allowed. Hollomon
with the change of hardness during
and consider
that the treatment
and
Section
1970
would not hold for aluminium
3 will
description
of ‘Lhardness.”
showed
18,
and steady
between havior.
In Section
the relationship
VOL.
components
that depend on the anelastic
together,
the description
in the
chosen, the mechanical state of a specimen after some further plastic deformation depends on the actual
present section may seem to the reader to be occasionally unfamiliar. Such problems, however, are easily
deformation
settled
path rather than only on the final state
when the recoverable
strain components
are
of strain relative to the reference state. Nevertheless, previous attempts at a rational description of plastic
added later. We proceed then to the consideration
properties, in particular those by Ludwikcl) and by Zener and Hol1omon.Q) have employed E, as a prominent stat’e variable. Measurements by Dorn et d.(3)
tical, purely plastic material whose properties we shall then show are not in disagreement with what is thus far known
of a hypothe
for the class of restricted
materials
HART:
PHENOMENOLOGICAL
THEORY
FOR
The description will be mad& in above. of plastic tensile strain E (we now drop the
PLASTIC
601
DEFORMATIOS
mentioned terms
subscript
p for simplicity),
stress IJ. The extension
E ,O
strain rate t, and tensile to multiaxial
deformation
will be reversed for a later publication. Of the three deformation variables 0, d and E, the two that are uniquely
indicative
state of the specimen the imposed
of the mechanical
are the first two, (T and g.
If
strain rate i is stated, the corresponding
.5
z L.2
stress G to produce d is a measure of the current state of mechanical
strength
mechanical
of the specimen.
In fact
the
state of the specimen at any instant is fully
specified by the set of all possible pairs of values of u and i of which it is immediately define
a property
(we employ
that
capable.
we shall
call the
5 .k4 .i
E 8 O
Temp
We shall
250°C fi 074 kgf/mmz 225’C
hardness
the term in the sense that one speaks of
strain hardening, and, of course, our term has nothing to do with a hardness indenter index) and shall assign it the parameter
symbol
y.
be evident later, there is a variety of assignments
that
can be made, and it will seldom be necessary to use it as a variable for computation.
Its property
is illust’rated by the state equation that at any current value of the hardness, u = o(y, P) The parameter
A 0.73 0 0.06
200’C* q
9‘O
(I)
y then orders a oneparameter
family
kgf/mm kgf/mm*
2
094 kgf/mm* 0 95 kgf /mm? 38
At this point we
shall not give it a definite number value, since as will
explicitly
7 ‘O
j
36
34
2
u/G
log
Influence of stress, u, on steadystat,e creep rate, E, of aluminium. For each plotted pomt the stress is normalized by dividing by the modulus att the temperature in question. Solid lines: present work. Each line refers to one specimen only, and the plotted points on each line give the succession of steady creep rates as stress reductions were made. Broken line: previous work. Each specimen was subjected to creep at a different constant load at 250°C. FIG. 2. Data plot from the work of Mitra and McLean. Ref. 4.
of aP relations of which one is always the characteri
then, if the stress is changed suddenly
stic a2 relation for a specimen at its current hardness.
plastic rate i, will be on the line that contains
In Fig. 1 we show schematically
There must be negligible plastic strain during the time
different
a
few such curves for
states of hardness of a single material.
definiteness,
and because
makes the assumption
the limited
reasonable,
For
data available
we represent them
as parallel curves with slope Y on a plot of log G vs.
of the measurement strain hardened neighboring
will have
so that it lies on a higher
line.
important
when loaded
they observed
at the rate C,,
or else the specimen
further
ol, d,.
Tests of this sort were carried out on Ni and Al in an
log &. The meaning of the curves is that if a specimen, at the stress ul, deforms
to a,. the neu
following They
study
by Mitra
and McLeanc4) in which
a series of relatively
successive
observed
steady strain rates
step reductions
in addition,
short time relaxation
process
below
an anelastic
is most
likely
of load in creep.
at each load change, which
a
we shall show strain
recovery
proportional to the stress change. Their observed values of C vs. (3 for Al are shown in Fig. 2. These are substantially the type of curve that we are characterising as curves of constant hardness. If a plastic equation of state of this form is to hold, it is necessary that, if two samples
that have undergone
different
strainstrain rate histories exhibit the datum point ul, i,, then both must, when the stress is changed to log i FIG. 1. Several lines of constant. hardness are shown schematically. For illustrative purposes they are represented as parallel, straight lines with a common slope Y.
02, strain at the same rate 6,. In other words it must not be possible for two constant hardness curves to intersect. All curves for a given material must be parallel.
There
is little data
available
to test this
ACTA
602
requirement.
Mitra and McLean
corresponding
did produce
to more than one initial
several temperatures essentially
RIETALLURGICA,
parallel.
curves
hardness
18, 1970
as the expressions
at
and obtained
curves that were
It is important
that their curves
are not parallel to the locus of points corresponding the usual data of stress vs. minimum creep rate.
VOL.
to In
y = (i3 In a/&).
(3)
and v
3
(i3
In o/a In &
It will be seen immediately
(4)
that. if a plastic equation
fact the slopes differ by as much as a factor of two.
of state of the form described
We shall discuss this work further in a later section.
exists, then v is the same as the slope at each point of the constant hardness lines of Fig. 1. and, further
To return to equation
(1) we see now that the pro
posal of Ludwik and of Zener and Hollomon combines the required behavior we have described above. and the
additional
assumption
that distinguishes
only of the accumulated present
work
that
the
parameter
is that,
strain
The point
E.
if this latter
that the resultant
of the
assumption
replaced by a more realistic kinetic equation, fair likelihood
y
one line from another is a function is
there is a
description
will be
more, v is then independent
in the previous
of history
section
and depends
only on the current value of a and P. The conditions
for the existence of a plastic equation
of state and a clue to its explicit form can be obtained of the integrability of the differential
by a discussion
form of equation (2). With a view to the desired form of the ultimatth relationship
we rewrite equation
successful.
(2) in the form
de=adlna+~dlnP
(5)
a = l/r
(6)
p =
(7)
where 4. THE
RIGOROUS
In this section
we proceed
strain hardening ways:
PHENOMENOLOGY
process.
(1) by describing
to a discussion
This can be done in two the rate of change
current flow stress as a function rate increments
or (2) by describing
of the
of strain and strain
(or. where it is pertinent,
change of .! as a function
of the
the rate of
of a and strain increment),
the rate of change of a suitably
selected hardness y as a function of any of the controlled deformation variables. Both procedures are equivalent,
We now seek the conditions
under which equat,ion (5)
possesses integral solutions
that are independent of the
path ofintegration.
If such solutions exist the differeu
tial form is a perfect differential. The first condition that must be satisfied
for
both procedures. All
the
deformation
interested
can
be
differential
form
histories
described
in which
incrementally
we
are
by
the
simply
(8)
v = v(0, i)
(9)
(8) and (9) are satisfied equation
known as a Pjaflall
describes
(2) the smooth
variation
of
any of the deformation variables in terms of the others. In general. the coefficients y and v at any stage in t,he deformation
If equations
7 = y(a. $)
process depend on the current values of at
least two of the variables previous deformation
a. E and 1 and also on the
history.
(
[email protected] Then if equation
In P), =
cap/a ItI ~1;
relation of the form E
=
z(a,
rather than a and d because of practical
This is the form of the Ludwil;
This
mon equation
employed
by
Hartt5’
in an earlier
same study
as that with t.he
that what was there called nl is here called
v. The reason for this change in notation is that, as we shall see below, there is more than one important rate sensitivity coefficient and the common use of the letters m or n does not make this distinction. For any particular deformation path, y and v can be identified
(11)
cr = a(E. C)
We choose In a and In d is the
F)
or equivalent1.v
simplicity.
description
(l(‘)
(10) holds there will exist a statci
as variables
difference
(5) is
,li)~j~ and it is directly integrable
if and only if
dlna=ydf+vdlnP This form
is that a
and b (and therefore y and v) be unique functions of cr and C. In other words y and v must be of the form
and both are useful.
We shall first develop t.he necessary background
v/y
(12)
and Zener and Hollo
of state, and again we see that it, in
volves two explicit requirement8s, viz. equations (8) and (9) and equation (10). Now. since equation (5) is a form in only two independent variables, the theory of Pfaffian
[email protected]) shows that. so longasat least equations (8)and (9) hold, and even ij equation (10) does not hold, there always exists an integrating factor of the form F(a, i) such
HART:
PHESOMESOLOGICXL
THEORT
that Fck=IxFdIncr+~FdIni
(13)
differential. The original Pfaffian form is then said to be int.egrable: and we can then write is a perfect
& = F & =aF(1!lna+PFdlni
(I2)
And so there exists a family of integral curves y = y(n. P)
(15)
where y can now be identified as what we called the hardness parameter. Furthermore, there is an infinite number of integrating factors and so the specific choice of y need not be unique although the curves are unique. Finally for each fixed value of y the corresponding curve given by equation (15) is a solution of the Pfafiun equation, dy = II
or, eq~~ivalent,l~, L2E= 0
(16)
and so all points along each integral curve are connected only by pat,hs for which de = 0 in consonance with our prescription in Section 3. Thus the integral curves satisfying equation (16) are our curves of eon&ant hardness. We can now summarize the out,come of this analysis as follows: A necessary and sufficient condition for the existence of a plastic equation of state is that y and v be functions only of u and 6 (at a single temperature). If the strain is to be a good state variable it is further necessary that equation (5) be a perfect differential. We shall now discuss the two procedures stated at the beginning of this section. The first procedure follows immediately from the satisfaction of the integrability requirement, equations (8) and (9). It is first necessar to determine by experiment whether those equations hold and then to determine their explicit form. Given t’hat this has been accomplished, equation (2) becomes rl In d = ~(a, &) de +
~(5.
t)
d
ln P
FOR
PLASTIC
DEFORMATIOS
603
necessary to select, among the many possible equiralent choices for y: one choice t,hat is well suited for both theoretical and practical purposes. The choice that we shall make is arrived at in the following way. If in equation (8) y is assigned a constant value. a locus of aC points is defined at each of which y has t,he same value. In particular if ae choose the locus y = 1. we have determined a curve at each point of which (au/a&); = (T (15) The point at which equat,ion (17) is satisfied is of course very nearly the point of plastic inst,ability in tensile deformation. Furthermore in the constant extension rate test it is substantial]> the point of load maximum. and in the constant load creep t,est it is the point of minimum strain rate. It is therefore a readily obtained and commonly available set of data. and it defines a log clog P curve that is substantially a straight, line. It is the slope of that, line that is commonly taken as the strain rate sensitivity. Furthermore, it is, in much of the current, lit,erature, loosely characterized as the steady state locus. The actual steady state locus, if one exists, is of course the line corresponding to y = 0. We shall have more to say on this last point later. We have plotted in Fig. 3 the curve y = 1 together with several curves of constant hardness. We assign the symbol p to the slope of the y = 1 curve. In general f~ > Y. Clearly, Fig. 3 is in complete agreement with t,hc data of Mitra and McLean shown in Fig. 2. The additional curves shown parallel to the y = 1 line are related t,o
f”‘)
and this differential equation can then be integrated over any prescribed deformation path to predict the mechanical behavior of the material. We shall do that in Section 5 for a variety of familiar test situations and for an assumed form of y and v. It can be seen that. even when E is not a state variable, it can still be handled as a path variable with no difficulty. It is o~easionally convenient to use the hardness y as an explicit stat,e variable. First. however, it is
Fro. 3. Schematic “equation of state” plot showing lines of constant y intersecting lines of constant y. The labelled dashed lines issuing from the paint o,, E, are the loci for the three deformation histories dtwcribrd in the text.
ACTA
604
METALLURGICA,
the assumed complete model we shall discuss below and are lines for other values of y. Since every constant hardness line intersects the y = 1 line we now choose the vaJue of Bat that intersection as the value of y. We could equally well have chosen the value of d at the intersection, but the choice given here is mathematically convenient. Note that the existence of such intersections means that a specimen at any hardness level whatsoever always can be made to exhibit a value ofy = 1 by choosing the correct value of d. In other words there is in principle always a test’ t,hat can be maclc to measure the current value of y, i.e. it has an operational meaning. We may now reduce the content of Fig. 3 to analytic form. If @i(P) is the functional form of the line y = 1, we have (ri = CC.? (13) where cc is a constant at any one temperature. It is easily verified that the equation for the line corresponding to any given value of y is (r = We
aypc_'iy
~)(a ln y/s);
18,
1950
as a complete function of 6, t and T. and this is not available from the existing data. We, therefore, adhere in the present paper to the parametric approach. The more general treatment, just described, will be explored further in a subsequent publication. 5. A
SPECIFIC
MODEL
In this section ne shall discuss the manner in which test. results are predicted within the framework of the theory set forth above. In principle. all deformation histories can be obtained from integration of equation (2’) once the functional forms of y and 1’ are known. For illustrative purposes we shall make an explicit. assumption about the nature of those functions. This assumption, of course, affects only the special form of the solutions in t,he examples considered below, whereas the general theory will admit an_vfunctional forms for y and v that are able t’o be determined experimentally or that, can be predicted by microscopic theory. Nevertheless, the author believes that the one used here is in fact appropriate to the simple f.c.c. metals. We postulate. then, that,
(19)
may note also that from its definition y = (1~
VOL.
v = constant
(22)
y = (q/o)“”
(23)
and (20)
Since y necessarily has the same value over any single integral curve, (a in y/i3 in d), E 0 and so the derivative in equation (20) can be replaced by a total derivative. Then
where bl is given by equation (18), and 1 is a constant with a value generally around i_ For clarity we recapitulate the other equations that are part of our model. dlno=ydsfvdlnP (2) 0, = a$’
(18)
There are for any given material four constant parameters in the model, viz. cc, ,u, v and il. and so as soon as we know how y depends on d and F: We shall now comput,r the resulting behavior for we know how y changes with strain increments. tests at, constant stress. constant strain rate and In t,he foregoing discussion we have maintained the stress relaxation at fixed extension. temperature T fixed. We now explicitly add the assumption that y is unchanged at T, by an excursion I. Comtant strain rate to another t,emperature T, followed by a return to T, This case, which is not exactly the same as constant so long as ds = 0 during the process. Then T will extension rate. yields. of course, the ideal tensile appear simply as a parameter and y, p, v and a will in stressstrain curve. Since e is constant.. equation (2) general depend on T parametrically. Because of our becomes mode of measuring y it will, even for a fixed state of d 111IT= y de (24) hardness, depend on T. It is possible, however, to and cri has t,he constant valuct given by equation (18). generalize our treatment so that T is treated explicitly Then as a stat’e variable. When that is done it is possible d In d = (~~~~)I’~de (25) to define the hardness state variable y in such a way that it is not temperature dependent just as it at We must still specify what the state of hardness of the specimen was when the straining commenced. At present is not strain rate dependent. That procedure, the value of 6 we employ this can be done by specifying however: requires the knowledge of the quantity the initial value of o or of y. However, if we wish to & = [a in a/@ l/kT)];,, compare identical specimens at several strain rates we Y = (P 
y)(d 1n y/de)
(21)
PHENOMENOLOGICAL
HART:
must know rate.
This
specifying
the corresponding is most
easily
values
done
by
THEORY
at each strain determining
or
the initial value of y. which is common
all the specimens, and employing determine
equation
We shall designate
(19) to then
the values of u, y and y when E = 0
as oo, y. and yo. We can readily integrate equation c = oJ(o&J1’i.
+
(25) to obtain
(26)
(18) and (19) yield (25)
~oo/$ = (Yoli.Y’”
of equation
value,
The
principal
features
we have computed displaced strongly
origin
(28)
(28) into equation
!
for the
the ostensible qualitative
strain
scale
that
depends
Note that the curve for “high temperature” rate.
Despite
differences in the curves, all
the same law, and none of them will
reach a steady state. II.
Constant stress For this case d In CY= 0, and equation
(2) becomes
O=yde+vdlnP Now from equation
(30)
(23)
(23) also
(&/41l
(29)
In order to make the result more concrete, (28) for assumed
values
we have
iz = 2~ =
4v = 0.2 for a few strain rates in Fig. 4. These values I
I
L2 I
1
a
curve
y = (oJo)l’~ = (a.Y/o)‘/”
y = [(yo/$P““‘.
equation
of the stressstrain
on the strain rate.
of them obey
simulates
rate.
is that it is a power law with a
gives the result
plotted
and this effect
spurious, high initial hardening
(26) in the explicit form
0 = cXd”[(yo/~)(PV)‘~ + (E/1)]” Substitution
to a low
605
DEFORMATION
curve with very low strain hardening
t,he result
and so we may write equation
PLASTIC
very low strain rate is a typical
(#IA
It is readily verified that equations
drops
to
the initial value of cr at each value of d.
FOR
(31)
If we express the applied stress CTin terms of d,, the strain rate that will be reached stress u, equation
when y = 1 at the
(31) can be written in the simpler
form y = (+#‘i”
(32)
where 8, is simply a measure of the applied stress and is given by d = ad,’ Now equation integration
(33)
(30) can be written in a simple form for
as d( E/V) =

(d/i,)‘‘Pl”’
d( i/i,)
(34)
If .G,is the initial value of the strain rate, this integrates readily to (6J8)“‘”
= &/i,)P’”
where 8, is given by equation 0’
0
I
I
RI
a2
hardness,
I
are not inconsistent moderate
with the data available
d =
temperatures.
this point to remember not to be compared
for Al at
The reader is cautioned that the curve deduced
immediately
at
here is
with an experimental
curve at constant extension rate. The reason is that the anelastic strain has not been included. That component affects only the first few per cent of strain since the plastic strain rates does not come up to its full value until the anelastic 4
strain rate contribution
(35)
(33) and, if yois theinitial
do is given by
RJ
FIG. 4. Constant strain rate tensile curves as conmuted from equation (28). The strain rate ratio betweenadjacent’curves is 10m4. The uppermost curve ISfor she lowest, strain rate. Note that+aeh wrve is plotted relative to the value of a at y = 1 *s unity.
+ (P/1V)&
ay~“~oy
(36)
The apparent shape of the curve of d vs. E is determined by the value
of the additive
given specimen
term
(i,/io)r”.
(i.e. for fixed yo) the value
For a of that
term depends strongly on the value of 0. Since p > v, the additive
term is small for large 0, and vice versa.
The two different
extremes
absence of sizable amounts
simulate
the presence
of “primary
or
creep”.
Since g = dsldt, equation (35) can be integrated once more to obtain E as a function of t. We present the result here for completeness. (P/d++
= [l +
(Yr)l‘wJ$)“‘A + (/4/ilV)&]lf’“‘“’  (+,)l+‘“‘“‘}
(37)
ACT.4
606
Although actually
this expression quite simple.
that at sufficiently
is somewhat
BIETALLURGICA,
messy,
It has the interesting
it is
$llta/a)l
(38)
In the stress relaxation testing
machine
test the crosshead
is held
interval of constant extension then continues influence
fixed
after
velocity.
of a
a prior
The specimen
to undergo plastic straining under the
of the
stress
due
strain in the specimen As the specimen
to the
residual
elastic
and the load measuring
extends
due to the relaxation
plastically,
cell.
the stress drops
of the elastic strain in such a
way that
Cji= _Ki. where K is the appropriate specimen
and machine.
will
be very
experience
during
small
and
history
a oi
for the
line of constant hardness.
the subsequent so the specimen
description
can be
has not yet been
believes
that
parameters
the
carried
temperature
of the theory
He anticipates
of K.
out,
the aut,hor
dependence
of
may be relatively
that the temperature
the
simple.
dependence
of
,u, v and ii may be only slight, and that the main variat.ion with temperature will be found for a and for the value of y for any given state of a specimen. 6. RELATIONSHIP
TO
EXPERIMENTAL
DATA
In order to discuss the relationship
of the proposed _ _ it is first necessary
theory to the results of experiments
to consider in a little more detail the effect of anelastic phenomena
in the experiments.
not to examine
t,he detailed
Our concern
here is
nat,ure of anelasticit,y
by Zener.“) Anelastic
The phenomenon
fully in the excellent
strain F, attendant
monograph
upon the application
of a stress ~7to a specimen can generally be characterized by laws that are linear in Ed, o and their time
of
equation
(39)
we obtain
directly
the two
derivatives.
The progress of E, with t’ime is generally
do = Kd&
(40)
and dlna=dlnC:
(41)
these mechanical
ships in equation
constraint
relation
(yU,/K)
d
ln u + Y d ln 6
a hard machine
111 ti)[l
+
(43)
K > a, and,
(43)
(yd/K)]
furthermore,
decreases rapidly, y also becomes quite small. fore. to a very good approximation
as 8 There
v = d In o/d In 6 The stress relaxation
(44)
test is then a very good
constant
hardness
curves
presented
test
and
complishes by a continuous variation what attempted by the discrete load change tests. The calculation
upon reduction
acwas
here does not include
constant, and (c) is
of cr. The relaxation
elastic relaxat,ion
can be as diverse as viscous
boundary
The physical
t.ime
basis for angrain
relaxation,
stress induced ordering of solut,es. and short distance displacement or bowing Since the effects can be produced
by
of dislocat’ion arrays in cell walls the magnitude
of
the effect can depend to some extent on prior plastic deformation
as well,
but at any outlined
one stage
it still
above and has no
direct relationship to the nature of the plastic straining process. It is essential, therefore, that the anelastic
strain
component
attempt,s
to
make
essentially
irreversible
be
detailed
identified
before
interpretation
of
one the
plastic component.
For illustrative purposes we shall show that the recovery time measured by Mitra and McLeanc4) can be explained quantitatively, entirely on the basis of an anelastic relaxation and no recovery of strain hardening. As related above, they deformed a tensile specimen
a
time
on o.
retains its basic properties
Y = (d ln o/d
one
does not depend
small displacements
or. solving for Y,
out
at, least
G at full relaxation,
that result from plastic deformation,
((Y/K)do+vdlnd =
to
of dislocations.
(2) to obtain
dlnu=
with
(b) proportional reversible
relationships
tracing
can be
(39) and a measurement
tal data
(a) exponemial
We substitut,e
data
analysis of the fit to experimen
will
our theory.
for
a detailed
of the fact’s of plastic deformation.
We shall now relate the t’est to the parameters
ln
ness by using equation
itself is discussed
found in Ref. 5.
From
the relaxation
his
that essentially follows a This test has been described
by several authors, and a detailed
of course,
but rather to show the way in which it can mask some
If K is large (a stiff machine)
the strain accomplished tory
(39)
elastic coefficient
curve for
reduced to an explicit plot of a vs. 6 at constant hardAlthough
Stress relaxation test
tensile
1970
of the early part of the relaxation
If desired,
which yields N3 when J. = 2~. III.
correction
18,
anelasticity.
feature
large values of t e_
T’OL.
in creep for an initial time interval
and then dropped the stress o1 by an amount Ao.
The
HART:
~HE~OME~OLO~ICAL
THEORY
strain rate then dropped abruptly to B very low value after which it gmdually rose to &new relatively steady value .+,that was less than the value il at the former stress or. They measured a time At that wss the interval from the time of stress change to the intersection of the time axis by s straight line dmwn through the straintime points when the strain rate had become steady. In other words, if t = 0 when the stress was changed, the strain as a function of t ultimately become asymptotic to 8(t) = &(t 
At)
(45)
Kow, if it is assumed that, upon the change ha, the plastic strain rate immediately becomes g,, and the anelastic recovery is A&,(t), the incremental strain after t = 0 would at all values of t be
c(t) = d,t + he,(t)
(46)
Furthermore AC, will after a relaxation time reach the value Ahe,= (LEG)lAho
(47)
where OLis 8 constant of the order of unity since relaxed anelastic moduli are comparable to the elastic moduli. Then, taking the value of equation (46) at large times and comparing it with equation (45) we see that Mitra and McLean’s At can be expressed as At = A&J& = AgluG~~
(48)
They then formed the quantity r that they termed the recovery rate as r/G = AolGAt
(49)
With our interpret&ion this is computed to be r/G = ad,
(56)
This last result agrees qu~nt~~tativel~ with their measurements. We see, therefore, that the At so determined has nothing to do with either stress recovery or even with the anelastio relaxation time. It is instead a measure of the ratio of the total anelastic recovery to the &ml strain rate. This point hss been discussed in detail because it has strong bearing on the interpretation of all experiments of this type. It should be easily possible in such experiments to measure the anelastic strain in the sbsence of appreciable plastic straining by interrupting the test by reverting to considerably lower stress levels. It should then be possible to observe the successive introduction and recovery of anelastic
FOR
PLASTIC
DEFORMATIOS
607
strain by repeated cycling between two stress holding levels. This in fact is what is occasionally done monotonically in the course of creep tests and is known as creep recovery. The large magnitude of the effect is discussed in the chapter on “anelastic creep” in the book by Lubahn and Felgar.ls) They shsw the dramatic change in the appearance of creep curves when the anelastict or recoverable. strain is measured and subtracted from the tot,al strain. The important modification occurs, of course? in the early part of the curve and makes the shape flatter. Substantially, the same phenomenon is present in the constant extension rate tensile test. Part, of the st,rain during the initial loading is anelastic and so the plastic strain rate does not rise to the vafue of the imposed strain rate until most, of the anelastic straining is concluded. The same phenomenon is probably responsible for the hysteretic behavior attendant on interrupted tensile testing in which straining is interrupted and the load reduced to zero followed by resumption of straining (cf. Ref. 8, chapter on Bauschinger effect). In order to be able to sort out the recoverable strain from the total strain it is necessary to collect data that will determine the nature of the anelastic behavior for each system with which one deals. The data from conventional tests csn then be analyzed to determine the character of the purely plastic strain behavior. It is, of course, the plastic behavior that the author believes will be susceptible to description by a theory of the form that has been developed above, We do not claim that there cannot be additional short time relaxation effects associated with the change of the plastic strain rate accompanying a stress change, but only that the effects associated with recoverable strain must first be accounted for before the remainder has been identified. In the case of the measurements of Mitm and McLean there does not seem to be tany remainder. We shall discuss other possible relaxations a bit further in Section 7. It is of further importance that, the data that is intended to elucidate grain matrix deformation properties, with which we are here concerned, should not have sizable contributions from grain boundary sliding. There is, after all, no reason to believe that a simple behavior or a single theoretical description will characterize data that represents composite phenomena. The marked effects that can be produced by grain boundary sliding were clearly exhibited by Servi and GrantJ9) and s,re even more dramatically evident in the current literrtture on “superplastioity”. Nevertheless, most of the high temperature data that is freely interpreted in terms of purely matrix flow
608
ACTA
METALLURGICA,
mechanisms lie wholly in the grain boundary sliding regime or in the transition range. This has obscured the understanding of the matrix deformation processes at elevated temperatures. It is in fact probable that those processes are not appreciably different from low temperature behavior even up to an appreciable fraction of the melting temperature. The data with which we are concerned, then, is for coarse grained specimens and generally at rather high strain rates or at moderate temperatures. There is reason to believe that, if we can adequately describe the matrix flow properties and the grain boundary sliding properties separately, then it will be possible to produce a theory that describes the combined operation of both mechanisms. An attempt at such a theory has been made by HartP”) for the presumed “steady state” behavior. A similar treatment should be possible for the entire strain hardening regime. We shall conclude this section with a brief discussion of the problem of the “steady state”. Considering the importance of the implications that arise from the existence of a steady state, it is amazing that its existence has been rather generally accepted with such slim experimental evidence. In tensile tests the specimen becomes unstable against necking as soon as y = 1. Certainly, no conclusion of a crucial nature can be drawn concerning the strain hardening rate beyond that point. It is not usually recognized that the constant nominal stress creep test is no better in this regard than the constant load test, and it does not have the built in indicator of the creep rate minimum to signal that point as the latter test does. Such tests in fact enter the range of instability quite as early as the constant load test and the apparent flatness of behavior at larger strains is misleading. Cavity formation at grain boundaries can produce further spurious strength reduction at large strains that has nothing to do with the matrix flow behavior. Finally, the putative steady state is generally identified by a guess that it has “almost been reached” rather than by a quantitative criterion. A simple reduction in strain hardening rate to some low value is not a sufficient characterization of the approach to steady state behavior as we have shown by our model above. Most theories that describe a steady state property imply a rate of approach to the steady state that is exponential in time or in the deformation path variable. In fact it is very hard to construct a theory that does not have such a prediction. There is absolutely no evidence of such behavior in the data for metal deformation. Even the tests of Taylor and Quinney(ir) in compression of copper
VOL.
18, 1970
showed considerable additional hardening beyond the point that is usually taken as the steady state and showed no cessation of hardening as far as the test was carried. Such behavior more nearly resembles the power law exhibited above rather than an exponential one. We claim, then, that there is no convincing evidence in the literature for the existence of a steady state regime. This point is not a trivial one since it has a profound effect on the nature of both phenomenological and microscopic theoretical description. Despite the strong wording of the foregoing paragraphs it is possible, as is shown in the next section, that many of the current theoretical ideas concerning the “steady state” creep may nevertheless have application in a broader context. We also note, parenthetically, that the existence of a steady state is not at all in contradiction with the general phenomenology of Section 4. If for example y(a, i) is of the form y = &[(U,/U)‘!“” 
l]
(51)
where 6, is the steady state stress given by 17,= a$’
(52)
and L1, A, and a, are constants, steady state behavior will be described. We do not pursue this further. 7. RELATIONSHIP
TO
MICROSCOPIC
THEORY
As claimed in the Introduction, a phenomenological theory can provide a proper framework within which to construct and test theories based on microscopic mechanisms. We shall now show that our theory implies some restrictions on theories that have not generally been recognized. In particular it has strong implications concerning the effect of the dislocation substructure that is developed during plastic deformation. In order to make the discussion concrete we shall present it in terms of the specific model of Section 5. However, it should be recognized that the features we are concerned with are actually properties of the general theory and do not depend on any specific functional form of y. We first rewrite equation (19) in a form that is more usual for microscopic theories as i =
~l/“a’/“y(“~)/v
(53)
Furthermore, from equations (18), (21) and (23) we may write the kinetic equation satisfied by y as d In y/d& = (p 
V)‘(d/y)“‘“”
(54)
Now any one value of y at a single temperature T
HART:
represents
PHEXOMENOLOGICAL
a fixed
hardness
and from the fundamental particular
configuration
state
THEORY
of the specimen,
standpoint
it represents a
of dislocation
in a special form that treated T as a parameter and of and had sorted out T as a
had been more detailed state
variable.
we
Thus, if we
would
have
found
a hardness
that was independent of T and 6 just as y of i. Now the point is that the existence
variable
is independent
theory
conclude,
operative,
theory
therefore,
that.
while
any
the theories that have been constructed
are incomplete
in addition.
and probably
they have frequently
been addressed
state property called
phenomenological
that
a theory
In the theory
of steady
dislocation
state creep by dislocation
the structure parameter
source density.
is addressed
is
in principle
to describing the constant structure or constant hardness lines and cannot be applicable to lines of constant y. The steady state theory for motion of jogged screw dislocations structure tions”.
of Barrett
parameter
and Nixo3)
the “density
That parameter
theory
however
lating
that
is in fact prescribed
to have
history.
does not contain
Furthermore,
parameter
a kinetic to
law re
deformation
the stress exponent
tions from the mobility
The
contribu
factor and from the structure
factor do not separately agree with the exponent differences between constant structure and constant y lines as measured by Mitra and McLean. theory of Johnston “dislocation dynamics” Gilman,
which
is the prototype
and Nix theory> also employs density
as a structure
theory that explicitly
for the Barrett
the mobile
parameter
The and
and
dislocation is the only
prescribes a history dependence
for the parameter. It is clear, in addition,
that the only steady
feature of the theories that are so characterized which has to do with the dislocation jixed
or prescribed
structure,
and
state is that
flow rate at any so
the
theories
actually neither predict nor require steady state behavior in the sense of saturation of work hardening as we discussed in the preceding section. The possible additional short time relaxations attendant upon stress or temperature changes, over and above those due to anelastic strain recovery, could in principle be computed from either of the “steady state”
deformation of the
It is that
C = i(a. 2. T)
(551
d.Z/da = f(& 2, T)
(5’31
where 2 is some dimension tion structure
or moment
of the disloca
that figures as a sensitive
element
the theory and as a well defined state variable.
of
Any
such theory can then readily be put into the form we have discussed above and will be capable of predicting all pertinent deformation histories. 8. CONCLUSIONS
state” line, and its
by separate measurements.
structure
as
disloca
different values along the “steady value is determined
employs
of mobile
matrix
and
is the
Since that parameter
treated as fixed, the theory
of metal
theory.
depends on the stress a and the structure y, and on T
climb of Weertman,02)
to
the wrong data. In general terms we may then state the form or shape
u and y.
on
too simple, and,
must take if it is to satisfy the requirements
through
of the
may be in some way
of y shows the existence of a well defined deformation that is the same as what is commonly The resulting strain rate d then “structure”.
than
only empirically.
proposed rate limiting mechanisms them
places stronger
on the form of the microscopic
We
to do
strain hardening as such.
those determined
of the theory
choice for a measure of y.
but they would clearly have nothing
with structural bounds
601)
DEFOR&IATIOS
Thus the phenomenological
As noted above, the parameter y has a value that depends on T even if the hardness state is unchanged.
our particular
PLASTIC
theories,
substructure.
This is only because of our development
FOR
We have plastic
concluded
equation
that there probably
of state
strain rate for the crystal
matrix
specimens
class
necessary of
of a restricted and sufficient
a hardness
state
exists a
for the stress and plastic in polycrystalline of materials.
conditions
variable
The
for the existence
have
been
deduced.
When such a state variable exists it can be identified with some strength determining location
substructure
of plastic deformation.
The kinetic
the hardness state variable relationship
of the dis
in the course
law followed
to strain hardening rates has been shown.
theories
that the current micro
differ in the way they relate to this
phenomenological
analysis.
In some way all of them
are incomplete
and some are not fully consistent
the restrictions
imposed
deformation
experimental
that the concept of steady
is presently
misapplied
data, and that the concept,
in which it is currently the theories.
with
by the phenomenology.
We have also concluded state
by
has been derived and its
We have further concluded scopic
property
that is developed
understood,
to
the
in the form
is irrelevant
to
9. ACKNOWLEDGMENTS
It is a pleasure to acknowledge the benefit of discussions with Drs. R. L. Fullman and T. A. Prater
610
ACTA
METALLURGICA.
of the General Electric Research and Development Center during the pursuit of this research. REFERENCES 1. P. LUDWICK, Elemente der technobgischen Mechanik. Julius Springer (1909). 2. CLARENCEZENER and J. H. HOLLOMON,J. appl. Phys. 17, 69 (1946). 3. J. E. DORN, A. GOLDBERG and T. E. TIETZ, Metal8 Technol. T.P. 2445 (1948). 4. S. K. MITRA and D. MCLEAN, Metal. Sci. 1. 192 (1967). E. W. HART, Acta Mel. 15, 351 (1967). :: I. N. SNEDDON. Elements of Partial Dzfferential Equations. McGrawHill (1957).
VOL.
18,
1970
7. C. ZENER, Eluaticity and Anelasticity of iUetuZ8. University of Chicago Press (1948). 8. J. D. LUBAHN and R. P. FELGAR, Plasticity and Creep of Metals. Wiley (1961). 9. I. S. SERVI and h’. J. GRAST, Trans. Am. Inst. Xin. Engrs 191,909 (1951). 10. E. W. HART, Acta Met. 15, 1545 (1967), also General Electric Research and Development Center Report No. 69C334. 11. G. I. TASLOR and H. QCISTE‘I, Proc. R. Sot. A143, 307 (1934). 12. J. WEERTMAX, .4SM Trans. 61, 681 (1968). 13. C. R. BARRETT and W. D. SIX. ActaMet. 13. 1247 (19fisJ 14. W. G. JOHXSTOS and J. .T. GILXAS. J. ap$. Phis.%; 1% (1959).